408
R. Shobha and R.S. Nema
Indian Institute
of
Science, Bangalore, India
INTRODUCTION
One of the major causes of failure of polypropylcne(PP) film high voltage capacitors is PD (partial discharges). PD can occur in the cavities or gas pockets formed due to variation in tightness of windings, improper impregnation and swelling of the film due to its interaction with the impregnating fluid.The effect of pressure and radial dimensions are important in small cavities mostly because system impregnation is done at low pressures and the cavity size gets reduced .It is probable that with time the cavity pressure will equilibrate with that of the surrounding ambient medium due to diffusion process.An attempt is made hcre to study the effect of cavity dimensions such as diameter (0.9 mm to 3.2 mm) and depth (40 pm to 200 pm) on the various I'D characteristics and the related breakdown of thin PP films.
EXPERIMENTAL
Electrical grade biaxially oriented PI' films of thickness 20 pm and 39.8 p n were cut as circular pieces of 110 mm diameter. Cavity was drilled in the 39.8
pm
film at its centre using a highspeed PCBdrilling machine.
The electrodes
used
were
2n/3
Rogowski profile uniform field brass electrodes of 58 mm overall diameter and 19 mm radius of curvature embedded in epoxy (to form
75
mm overall diameter and 20 mm overall thickness) except for the flat portion of the electrode surface (exposed effective diameter of the electrode being 48 mm). The sample consisted of three layers
 the top and bottom layer each of
20 pm thickness in contact with the high voltage and ground electrode respectively and the middle layer having a cavity whose diametcr/dcpth is varied.
A
matching unit consisting of an RC circuit (R: coupling capacitor
(600
pF, 30
15GUl2,
C:
1000

150
pF), a kHz), power frequency filters at the input and output of the amplifier, an oscilloscope, and other necessary instruments were used for detcction and measurement of discharges. The sensitivity of detcction was 1 pC with a sample capacitance of
1OOpF.
Elcctronic counters were used for pulse height analysis.
The inception and extinction voltages wcre measurcd. The discharge pulse magnitudes and their repetition rates were measurcd once in four minutes over a period of one hour. The breakdown characteristics of the samples were obtained by the stepstress method. The voltage was raised
409 from lo00 V upto final failure of the sample in steps of 500 V, and held at each step for a finite time interval. The steptime intervals were 10 minutes,
5 minutes,
3
minutes and 1 minute. The total time for failure was recorded using a microsplitsecond digital timer.
RESULTS
AND
DISCUSSIONS
The inception voltage increases with decreasing cavity diameter for a given depth and increasing cavity depth for a given diameter. The first measurement gives the highest value for inception voltage and subsequent measurements show a reduction in the inception voltage finally stabilizing at a specific value. This stabilized value Vi, bears a definite relation to the diameter and depth of the cavity (Fig. 1) and is given by,
Vi
=
A
(d/rYB Volts
Where
A
and
B are constants, d the cavity diameter,
f
the cavity depth.
The extinction voltages are
12
to 20 voltage.
per
cent lower than the inception
Since the charge in the gas discharge avalanche must build to a minimum level within the dimensions of the cavity, a relationship exists between the minimum breakdown voltage or the inception voltage and the cavity dimensions (equation 1). When discharges occur in a cavity, the conditions in it may get modified due to the wall charges deposited, which may cause an increase in the probability of finding initiating electrons capable of developing critical avalanches due to field distortions. Also it is probable that products of ionization in the air produced by previous discharges cause a reduction in the breakdown voltage
so
that the initial inception voltages are the highest. Further, the fact that ultimately inception and extinction voltage stabilize at definite values suggests that the dielectric surface attains a certain optimum charge distribution.
Measurements of discharge magnitudes indicate that a single discharge does not completely discharge the entire cavity. The discharge pulse magnitudes, number and their distribution depend on the diameter as well as depth of the cavity. With time, the rate of change in discharge quantities is less in a smaller diameter cavity. The accumulative repetition rate against apparent charge shows an exponential distribution as compared to an ideal rectangular distribution.
Experimental and calculated values of maximum discharge magnitude for different diameters and depths of the cavity indicate that there is an increasing deviation between the calculated and experimental values as the cavity diameter increases (Table 1). This implies that only a part of the cavity and not the whole of it discharges. It must be said that this conclusion is based on the assumption that the cavity becomes
410 conducting after the discharge i.e. the voltage drop across the cavity is equal to the breakdown voltage of the cavity. Hence the effective diameter for the discharge can be calculated as follows,
Effective diameter of the discharge, deffectwe
= dcavity [
Qexpermental
/
Q c a l d a where Q is the charge magnitude
tcdl
Y2
,421
The effective diameters of discharge calculated are bctwccn 0.50 mm and
0.83 mm. The increase in the effective diameter with increasing diameter of the cavity is probably due to increased capacitance and hence the stored energy
.
In samples with larger cavity diameter the area available for discharges is large. The discharges occur preferentially between sitcs which are devoid of the effect of surface charges left behind by previous discharges.The discharges can follow paths of successively increasing lengths. Hence the number of smaller as well as larger magnitude pulses are higher. It is expectcd that for larger cavity diameter, a single discharge can cause wall charges to collect only on certain areas of the cavity wall facing the channel and not all over the wall. This should explain for the greater variation in the numbcr of pulses with increasing cavity dimension3 is probable that the greatest discharges occuring between the central parts of the cavity or tangential are less affectcd by the wall charges and hence vary less with time. The variations in discharge quantities with time could also be due to changes in the gas pressure as well as composition of the discharge products.
The inverse powerlaw model has been frequently uscd to estimate lifetimes of insulating materials under voltage stress. In the simplest form this model is represented by the equation, t(E)"= k
..
(3)
where
t
is the time to failure at voltage stress E, 'n' and
'k'
are constants.
Starr and Endicott 111 propoxd the concept of equivalent damage to estimate the life at constant stress from that on linearly increasing progressive stress. They found that the data fit a straight line on a loglog paper for progressive stress and hence suggested the applicability of inverse powerlaw model for progressive strcss also. Assuming a similar cumulative nature of damage to the insulation for the stepstress, the cumulative damage will be sum of the damages at each voltage Ievel, given by, t(E)"
=
Cts (Es)"
+
tstl
(Estl)"
..
(4)
tsEs is a product of time and voltage
stress
at each fully completed step,
tsti
is the time to failure on the uncompleted equations
(3)
and
(4)
indicate that the right hand side of equation
(4)
is a constant and is independent of the time interval ts chosen, provided
41 1
the ageing mechanism has not changed over the covered range. The advantage of using the stepstress method is that the times to failure is considerably reduced [21.
The breakdown stress against time to failure, Et characteristics, is shown in Fig.2. The 'n' values obtained from these curves are tabulated in
Table2. The 'n' values as well as the discharge quantities vary with cavity dimensions. An attempt has been made to fit an equation of the form n
= A' expB(Qm), where A' and B are constants and Qm is the maximum discharge magnitude. On extrapolation, this equation gives 'n' value of
11.3 for a permissible discharge magnitude of 10 pC. Krishnan and Nema
[3] in their work on surface PD ageing of PP films have obtained 'n' value corresponding to 10 pC as 11.8. The total discharge quantity/second
8
t
upto failure correlates with the time to failurdl) in the form L=a(Qt) and is shown in Fig.3. This indicates that Qt seems to be an important factor in the degradation of PP films. This aspect falls in line with the observations of Krishnan and Nema [3] where a similar relation for L and Qt is obtained for surface discharge studies, and of
Dakin [4] where it is stated that the rate of material degradation is proportional to the total number of discharges per second. It has also been found that for a given diameter and depth of the cavity, the
'k'
values corresponding to 10 minutes, 5 minutes, 3 minutes and 1 minute steptime intervals are all of the same order. Hence this suggests that the stepstress method can be used for a quick determination of the constants of the inverse powerlaw model for life characteristics in the presence of
PD.
REFERENCES
W.T. Starr and H.S. Endicott :"Progressive Stress A New Accelerated
Approach to Endurance", Trans. AIEE, PAS 80, 1961,
575.
P. Cygan and W. Khcchen: "A Short Method
of
Estimating Lifetime of Polypropylene Film using StepStress Tests",
IEEE Trans. on Elec. Insul.
25(6),
1990, 1180.
V. Krishnan and R.S. Nema
:
"A Study of Shortterm Partial
Discharge Ageing of Polypropvlene Film", IEEE Trans. Elec. Insul.
24(6), 1989, 1133.
T.W. Dakin
:
"Theory of Voltage Endurance", Addendum to Conf.
Proc. CEIDP, 1984.
ACKNOWLEDGEMENTS
Thanks are due to the authorities of Indian Institute of Science and
Central Power Research Institute, Bangalore, India, for granting permission to publish this work.
412
400
0 20
C W
40
60
DWM€TER/WW DEPTH
80
100
Fig. 1
:
Variation of inception voltage with cavity diametcr/dcpth.
Table 1
:
Calculated values of Maximum
Dischame Magnitude
Cavity depth
(pm)
Cavity diameter
(mm)
0.9
(pC)
198
“ld
QUI
0.31
40 2.0 976 0.13
Table 2
:
powerlaw modcl
Cavity diameter
 mm
Cavity depth
(um)
,
.
80
0.9
9.02
2.0
9.23
3.2
8.88
120
_ _ _ _ _ _     _  
0.9
330

0.40
200
7.03
5.59
5.99
5.53
6.60
6.50
120 2.0
0.9
1631
434
0.11
0.05
0.40
200 2.0
3.2
2142
5483
0.10
0.04
~~~
3.50
3.00
2.00
'0
Fig. 2
:
Effect of cavity dimensions on the Et characteristics.
413
0
400
TOTAL DlSCHbRGE
800
MACNWM
1200
(QtPC/aH)
1
)OXlOl'
Fig. 3
:
Variation of time to failure with total discharge magnitude.